- Nano Express
- Open Access
Humate-assisted Synthesis of MoS2/C Nanocomposites via Co-Precipitation/Calcination Route for High Performance Lithium Ion Batteries
Nanoscale Research Letters volume 13, Article number: 129 (2018)
A facile, cost-effective, non-toxic, and surfactant-free route has been developed to synthesize MoS2/carbon (MoS2/C) nanocomposites. Potassium humate consists of a wide variety of oxygen-containing functional groups, which is considered as promising candidates for functionalization of graphene. Using potassium humate as carbon source, two-dimensional MoS2/C nanosheets with irregular shape were synthesized via a stabilized co-precipitation/calcination process. Electrochemical performance of the samples as an anode of lithium ion battery was measured, demonstrating that the MoS2/C nanocomposite calcinated at 700 °C (MoS2/C-700) electrode showed outstanding performance with a high discharge capacity of 554.9 mAh g− 1 at a current density of 100 mA g− 1 and the Coulomb efficiency of the sample maintained a high level of approximately 100% after the first 3 cycles. Simultaneously, the MoS2/C-700 electrode exhibited good cycling stability and rate performance. The success in synthesizing MoS2/C nanocomposites via co-precipitation/calcination route may pave a new way to realize promising anode materials for high-performance lithium ion batteries.
Due to their high energy density, long cycle life, and environmental friendliness, lithium ion batteries (LIBs) are widely utilized in portable electronic devices  (e.g., mobile phones and watches), electric vehicles [2, 3], and renewable energy storage [4,5,6,7,8]. Graphite is the most widely used anode materials in commercial LIBs, benefiting from its low working voltage, good conductivity, and low cost [9,10,11]. However, the characteristic structure of graphite leads to feasible generation of LiC6, allowing only one lithium ion intercalation in every six carbon atoms which results in a low theoretical specific capacity of 372 mAh g− 1, which is far away from the current business requirements .
Currently, it is preferred to obtain appropriate electrode materials in LIBs for higher battery capacity, longer cycle life, and better rate capability. Consequently, Li-alloy-based anode materials , transition metal oxides , oxysalts, and transition metal sulfides  are often served as the anode materials in LIBs, since these materials display all the necessary properties for appropriate electrode materials. Among these materials, transition metal sulfides (e.g., CuS2 , WS2 , and MoS2 [18,19,20] have been an exciting topic in research as they are earth-abundant and show high specific capacity when used as anode materials in LIBs . As a typical representative, MoS2 has gained a lot of attention due to its particular S-Mo-S layered structure , high theoretical specific capacity compared to traditional graphite anode, and there is a transfer reaction of four electrons when used as anode materials in LIBs [23, 24]. In addition, the van der Waals forces between the MoS2 layers are very weak, allowing lithium-ion diffusion without causing significant volume change [25, 26]. However, MoS2 is still an unsatisfactory anode material due to its low electrical conductivity, leading to the poor cycling and rate performance . To solve this problem, a number of strategies have been developed to improve its electrical conductivity such as the incorporation of MoS2 with carbon materials [28,29,30].
To date, a variety of MoS2/carbon composites have been synthesized as anode materials in LIBs, namely, layered MoS2/graphene composites , MoS2/C multilayer nanospheres , MoS2-CNT composite , multilayered graphene/MoS2 heterostructures , or petal-like MoS2 nanosheets space-confined in hollow mesoporous carbon spheres . Despite gratifying progress in electrical conductivity, cycling, and rate performance of the electrode, some other conflicts in the synthesis method have persisted. At present, the most commonly used synthetic method is hydrothermal approach followed by an annealing process, which can introduce carbon matrix with some surfactants such as sodium oleate or oleyamine and sulfur element with some L-cysteine in the first procedure. Moreover, expensive and toxic organic reagents were always indispensable and unavoidable during the synthesis process when compared with co-precipitation method. Currently, co-precipitation method is just beginning to gain popularity in the synthesis of inorganic nanostructured materials due to its cost-effective, non-toxic, trustworthy, and stable [36, 37]. To the best of our knowledge, there has been little report on the synthesis of MoS2/C nanocomposite by co-precipitation/calcination process, especially with potassium humate.
Potassium humate, a sort of aromatic hydroxy carboxylate, which consisted of a wide variety of oxygen-containing functional groups, can be considered as functionalized graphene candidate . In general, a great deal of researches have been made to use potassium humate as carbon source to synthesize carbon materials under extremely harsh conditions [38, 39]. Huang  reported that potassium humate can be straightforward carbonization to prepare reduced graphite oxide materials. In this paper, MoS2/C nanocomposites were synthesized via a co-precipitation/calcination route, by employing an organic matter (potassium humate) and an inorganic substance ((NH4)6Mo7O24) as reagents. The electrochemical performance of the samples as a LIBs anode was measured, and the results showed that the sample calcinated at 700 °C (MoS2/C-700) exhibited better cycling ability and rate behavior. The discharge capacity of the sample remained at 554.9 mAh g− 1 after 50 cycles at the current density of 100 mA g− 1, which is much better than the other two samples calcinated at 600 °C and 800 °C, respectively. Meanwhile, the as-prepared MoS2/C-700 displays a comparable electrochemical performance [40, 24].
Potassium humate was obtained from Double Dragons Humic Acid Co., Ltd. Xinjiang (China), and the composition analysis of potassium humate was shown in Additional file 1: Table S1. All of the chemical reagents (except potassium humate) were of pure analytical grade and used without further purification.
Synthesis of MoS2/C
The precursor was prepared by co-precipitation from (NH4)6Mo7O24 and potassium humate in the presence of HNO3 followed by a freeze-dried process for 2 days. In a typical procedure, 4 g of potassium humate were dissolved in 40 mL of 0.25 M (NH4)6Mo7O24 solution. Subsequently, the above-mentioned solution was added dropwise to 100 mL of 0.5 M HNO3 solution with vigorous magnetic stirring. The duration of the magnetic stirring was for several hours. The lower precipitation was then separated from the mixture solution, freeze-dried, and labeled as Mo-HA precursor. The precursor was mixed with anhydrous Na2SO4 (with a proportion of 1:10) and ground in a mortar to form a homogeneous mixture. The mixture was then calcinated at 700 °C for 3 h (with a heating rate of 10 °C min− 1) and then naturally cooled down to room temperature. Finally, the products were washed with deionized water and ethanol three times followed by a freeze-dried procedure to obtain the MoS2/C powder. In parallel, the samples calcinated at 600 and 800 °C were synthesized as well.
The surface organic functional groups of potassium humate were measured by Fourier transform spectrophotometer (FT-IR, VERTEX 70, Bruker) with KBr as the reference sample. The structure and morphology of different samples were characterized by X-ray diffraction (XRD, BRUKER D8 Advance) with Cu Kα radiation (λ = 1.54178 Å), transmission electron microscopy (TEM, Hitachi H-600), high-resolution transmission electron microscopy (HRTEM, JEM-2100F), LEO 1450VP scanning electron microscope (SEM), energy-dispersive X-ray spectrometer (EDX), and X-ray photoelectron spectroscopy (XPS, ESCALAB 250Xi spectrometer). Thermogravimetric analyses (TGA) were conducted on a thermogravimetric analyzer (Netzsch TGA 409). Raman spectrum was carried out on Bruker Senterra with 532 nm wavelength.
Electrochemical measurements were performed on coin cells. The working electrodes were fabricated by mixing 80 wt.% of the as-prepared MoS2/C active materials, 10 wt.% of acetylene black, and 10 wt.% of polyvinylidene fluoride (PVDF) in N-methyl-2-pyrrolidinone (NMP) solvent to form a homogeneous slurry. The slurry was coated on the copper foil and dried in a vacuum at 110 °C for 12 h. The coin cells were assembled in an argon-filled glovebox. In the measurement, lithium foil was used as the counter electrode and reference electrode, and a polypropylene film (Celgard-2400) was used as a separator. The electrolyte solution was 1 mol L− 1 LiPF6 in ethylene carbonate (EC), dimethyl carbonate (DMC), and diethyl carbonate (DEC) (EC/DMC/DEC, 1:1:1, volume ratio). The galvanostatic charge-discharge measurements were performed in a potential range of 0.01–3.0 V by using a LAND CT2001A battery testing instrument (Wuhan) at room temperature. Cyclic voltammetry (CV) measurements were performed on an electrochemical work-station (CHI 660D) at a scanning rate of 0.1 mV s− 1 between 0.01 and 3.0 V.
Results and Discussion
The surface chemistry of potassium humate was studied using FTIR spectrum. In Fig. 1a, the broad peaks centered at 3400 cm− 1 were ascribed to the stretching vibrations of −OH, −COOH, and H2O bonds, The peaks at 1627, 1413, and 1050 cm− 1 were attributed to the stretching vibrations of the −COO groups and −CH, −OH and so on , respectively, indicating the rich oxygen-containing functional groups on the surface of pure potassium humate, which is beneficial to complexation reaction or adsorption. TGA curve of the homogeneous mixture of Mo-HA precursor and anhydrous Na2SO4 (with a proportion of 1:10) in an argon atmosphere with a heating rate of 10 °C min− 1 is shown in Fig. 1b. It can be seen that there are three steps of weight loss in the TGA curve. The first weight loss is 1.59% from room temperature to 250 °C, which may be due to decomposition of the water in the surface of the Mo-HA precursors. There are another two consecutive steps of weight loss, with a weight loss of 1.35% from 250 to 500 °C, and a weight loss of 3.17% from 500 to 800 °C, and then the mass remains constant, indicating that the precursor has been decomposed completely at 800 °C. For such a system, we choose those three temperatures for calcination as 600, 700, and 800 °C, denoted as MoS2/C-600, MoS2/C-700, and MoS2/C-800, respectively.
According to the literature , a possible mechanism of the reaction process has been proposed and schematically depicted in Scheme 1. Moreover, the corresponding formulas are listed in Additional file 1: Equations 1–5. In these equations, potassium humate was abbreviated as K-HA. There might be a complexation when potassium humate was dissolved in (NH4)6Mo7O24 solution, with the participation of HNO3 solution, which leads to the generation of Mo-HA. After heating the mixture of the Mo-HA precursor and anhydrous Na2SO4 in an argon atmosphere at a relatively high temperature, the Mo-HA precursor would be carbonized to form the intermediate of amorphous carbon, and then the intermediate would reduce anhydrous Na2SO4 to generate Na2S, further hydrolyzed to hydrogen sulfur. Finally, hydrogen sulfur may react with MoOx, leading to the formation of MoS2/C nanocomposites.
Figure 2a–b show the XRD patterns and Raman spectra of the MoS2/C nanocomposites calcinated at different temperatures. Figure 2a shows that almost all the diffraction peaks of MoS2/C-600 and MoS2/C-700 can be well indexed to the hexagonal MoS2 phase (JCPDS card no. 86-2308), which is consistent with those of previous report . There are still some other peaks mismatching the standard card in the MoS2/C-800 sample. We speculate that the crystalline of MoS2/C has been destroyed at high temperature. From the Raman spectra (Fig. 2b), it can be seen that the peaks located in between 379 and 400 cm− 1 belonged to E1 2g (the in-plane displacement of Mo and S atoms) and A 1g (out-of-plane symmetric displacement of Mo and S atoms) Raman modes, respectively [24, 43]. The bands appeared at 1347 and 1589 cm− 1 were the characteristic D- and G-band, and the value of I D /I G were 0.96, 0.91, and 0.94 as the temperature goes from 600 to 800 °C. The former corresponds to the amorphous carbon or sp3-hybridized carbon (D-band), and the latter assigned to the sp2-hybridized carbon (G-band) . Although there is no great distinction between the degree of graphitization, the MoS2/C-700 sample is still a little higher than the other two samples to a certain extent, indicating that the carbon in this sample is not only in the form of amorphous carbon, but also some graphitic carbon. Therefore, we focused on the MoS2/C-700 sample in the following investigations.
To further study the chemical composition and chemical bonds of MoS2/C-700, X-ray photoelectron spectroscopy (XPS) analysis was carried out. The survey XPS spectrum (Fig. 2c–f) reveals the presence of Mo, S, C, and O elements in the MoS2/C-700 nanocomposite. The high-resolution XPS spectra of Mo 3d and S 2p are shown in Fig. 2d, e, respectively. The peaks at 229.4 and 232.6 eV are assigned to the Mo 3d5/2 and Mo 3d3/2, confirming the existence of Mo in MoS2/C-700 [45, 46]. The presence of another XPS peak at 226.5 eV is indexed to S 2 s, which is resulted from the surface of the MoS2/C-700 . Moreover, the XPS peaks at 162.3 and 163.4 eV in S 2p spectra are characteristic peaks of the S 2p3/2 and S 2p1/2 of MoS2, respectively. Figure 2f shows that the C1 s spectrum can be divided into three peaks, denoted as C–C, C–O, and C=O groups, respectively.
The EDX spectrum indicates that the sample calcinated at 700 °C contains Mo, S, and C elements, as shown in Fig. 3a. Figure 3b, c show the SEM images of the sample of MoS2/C-700. For comparison, the SEM images of MoS2/C-600 nanocomposite and MoS2/C-800 nanocomposite were also shown in Additional file 1: Figure S1. In order to explore the corresponding element distribution in the sample of MoS2/C-700, the corresponding elemental mapping analysis were carried out. As shown in Fig. 4a–d, the elemental mapping images of MoS2/C-700 demonstrated the uniform distribution of Mo, S, and C all over the MoS2/C-700 nanocomposite, which is consistent with the EDX and XPS results.
As displayed in Fig. 4e–h, the morphology and structure of the as-synthesized MoS2/C nanocomposites were investigated by transmission electron microscopy (TEM), selected area electron diffraction (SAED), and high-resolution transmission electron microscopy (HRTEM). The TEM image (Fig. 4e) and the SEM images (Fig. 3b, c) clearly show that the structure of MoS2/C-700 nanocomposite is wrinkled two-dimensional nanosheets with the width of ~ 800 nm and the thickness of ~ 20 nm. SAED pattern in Fig. 4f shows that the hexagonal lattice structure of MoS2 is well crystallized. Furthermore, the crystal lattices of the sample were shown at HRTEM profiles ((Fig. 4g, h) and Additional file 1: Figure S2). The profiles showed highly crystalline MoS2 nanosheets with an interlayer distance of 0.27 nm corresponding to (100) plane of hexagonal MoS2 [24, 34]. In addition, Additional file 1: Figure S2 clearly reveals that the carbon nanosheets were decorated with MoS2 nanosheets.
Figure 5a shows the CV curves of the first 3 cycles of MoS2/C-700 electrode at a scan rate of 0.1 mV s− 1 in the potential window of 0.01–3.00 V vs. Li+/Li. During the first cycle, the reduction peak at 1.0 V indicates the lithium insertion mechanism, which is due to the insertion of lithium ions into the MoS2 layers to form LixMoS2. At the same time, there has been a phase transition from 2H (trigonal prismatic) to 1T (octahedral) . Another reduction peak at 0.4 V is attributed to the conversion of LixMoS2 into metallic Mo and Li2S. The broad oxidation peak located at 2.35 V represents the deintercalation of Li2S to S. During the subsequent cycles, the two cathodic peaks at 1.0 and 0.4 V disappear with appearance of three new peaks at 2.0, 1.2, and 0.3 V, indicating the reduction of MoS2 and the conversion from S8 to polysulfides and then to Li2S .
The discharge and charge curves of the first 3 cycles of MoS2/C-700 electrode were recorded, and the corresponding results were shown in Fig. 5b. In the first cycle, the discharge and charge capacities of MoS2/C-700 electrode are 802.8 and 651.4 mAh g− 1, respectively, with a Coulomb efficiency of 81.14%. The irreversible capacity loss may be due to some irreversible reaction such as the decomposition of electrolyte and the formation of solid electrolyte interface (SEI) film [49, 50].
The cycle stability of whole MoS2/C electrode and the pristine MoS2 electrode at a current density of 100 mA g− 1 are presented in Fig. 5c. At the same time, the Coulomb efficiency of MoS2/C-700 is also recorded. After 50 cycles, the discharge capacities of MoS2/C-600, MoS2/C-700, MoS2/C-800, and pristine MoS2 electrode at a current density of 100 mA g− 1 remain at 399.7, 554.9, 245.7, and 332.9 mAh g− 1, respectively. As shown in Additional file 1: Table S1, it has summarized the discharge capacities after 50 cycles of MoS2-based electrode presented in other literature, the as-prepared MoS2/C-700 display a comparable electrochemical performances compared to the previous work. It is concluded that the MoS2/C-700 electrode shows the most outstanding cycle performance and the Coulomb efficiency of the sample maintained a high level at about 100% after the first 3 cycles. It may benefit from the small amount of graphitic carbon in this sample, leading to enhanced electrical conductivity of the nanocomposite.
In addition to the cycling stability, the high-rate performance is also an important factor for high-power applications. Figure 5d shows the rate performance of MoS2/C and the pristine MoS2 electrode at the current densities ranging from 100 to 1000 mA g− 1. At 1000 mA g− 1, the discharge capacity of MoS2/C-700 can still maintain at a relatively high value of ~ 450 mAh g− 1, which is higher than the other MoS2/C electrodes and pristine MoS2 electrode we have prepared at the same current density. When the current density is changed back to 100 mA g− 1, the capacity of MoS2/C-700 sample can recover up to ~ 500 mAh g− 1 after 50 cycles at different current densities, revealing the good rate capability of the sample.
The electrochemical impedance spectra (EIS) measurements on the MoS2/C and the pristine MoS2 electrode were conducted in order to gain a further understanding about the excellent electrochemical performance of the MoS2/C-700 sample (Fig. 6). There is a semicircle at the high frequency region followed by a slope line at the low frequency region on these Nyquist plots. It can be seen that the semicircle at the high frequency region of the MoS2/C-700 sample is evidently smaller than that of the other three samples, which is related with the charge transfer resistance (Rct) occurred at the electrolyte and electrodes interfaces. Therefore, this result further implies that the incorporation of potassium humate markedly improve the conductivity of MoS2, leading to further improvement in the electrochemical performances.
In this work, two-dimensional MoS2/C nanosheets were successfully synthesized via a co-precipitation/calcination route by employing an organic matter (potassium humate) and an inorganic substance ((NH4)6Mo7O24) as reagents. Structural characterizations show that as-prepared MoS2/C-700 nanocomposite is two-dimensional (2D) MoS2/C nanosheets with irregular shape. The 2D MoS2/C nanosheets exhibited improved electrochemical performance when fabricated as anode material for LIBs. Furthermore, a possible reaction process was proposed. The current synthesis strategy may be expanded into the synthesis of other nanocomposite that can be served as anode materials for high-performance lithium-ion batteries.
Diethyl carbonate (DEC)
Energy-dispersive X-ray spectrometer
Electrochemical impendence spectroscopy
Fourier transform spectrophotometer
High-resolution transmission electron microscopy
- I D :
The intensity of D-band
- I G :
The intensity of G-band
Lithium ion batteries
MoS2/C nanocomposite calcinated at 600 °C
MoS2/C nanocomposite calcinated at 700 °C
MoS2/C nanocomposite calcinated at 800 °C
- R ct :
Charge transfer resistance
Scanning electron microscope
Transmission electron microscopy
Wang J, Yang N, Tang H, Dong Z, Jin Q, Yang M, Kisailus D, Zhao H, Tang Z, Wang D (2013) Accurate control of multishelled Co3O4 hollow microspheres as high-performance anode materials in lithium-ion batteries. Angew Chem Int Ed 52:6417–6420
Zou Y, Hu X, Ma H, Li SE (2015) Combined state of charge and state of health estimation over lithium-ion battery cell cycle lifespan for electric vehicles. J Power Sources 273:793–803
Wu C, Tong X, Ai Y, Liu D-S, Yu P, Wu J, Wang ZM (2018) A review: enhanced anodes of Li/Na-ion batteries based on yolk-shell structured nanomaterials. Nano-Micro Lett 10:40
Armand M, Tarascon JM (2008) Building better batteries. Nature 451:652–657
Kang B, Ceder G (2009) Battery materials for ultrafast charging and discharging. Nature 458:190–193
Xin T, Feng L, Jiang W, Wang ZM (2016) High performance perovskite solar cells. Adv Sci 3:18742–18745
Xie J, Liu L, Xia J, Zhang Y, Li M, Ouyang Y, Nie S, Wang X (2018) Template-free synthesis of Sb2S3 hollow microspheres as anode materials for Lithium-ion and sodium-ion batteries. Nano-Micro Lett. 10:12
Cao X, Shi Y, Shi W, Rui X, Yan Q, Kong J, Zhang H (2013) Preparation of MoS2-coated three-dimensional graphene networks for high-performance anode material in lithium-ion batteries. Small 9:3433–3438
Kamali AR (2016) Eco-friendly production of high quality low cost graphene and its application in lithium ion batteries. Green Chem 18:1952–1964
Xing X, Yu GH, Liu N, Bao ZN, Criddle CS, Yi C (2012) Graphene-sponges as high-performance low-cost anodes for microbial fuel cells. Energy Environ Sci 5:6862–6866
Luo R, Lv W, Wen K, He W (2018) Overview of graphene as anode in lithium-ion batteries. J Electron Sci Technol 16:57-68
Li HH, Yabuuchi N, Meng YS, Kumar S, Breger J, Grey CP, Yang SH (2007) Changes in the cation ordering of layered O3 LixNi0.5Mn0.5O2 during electrochemical cycling to high voltages: an electron diffraction study. Chem Mater 19:2551–2565
Mn O, Vl C (2014) Alloy negative electrodes for Li-ion batteries. Chem Rev 114:11444–11502
Reddy MV, Subba Rao GV, Chowdari BV (2013) Metal oxides and oxysalts as anode materials for li ion batteries. Chem Rev 113:5364
Xu X, Liu W, Kim Y, Cho J (2014) Nanostructured transition metal sulfides for lithium ion batteries: progress and challenges. Nano Today 9:604–630
Han F, Li WC, Li D, Lu AH (2014) In situ electrochemical generation of mesostructured Cu2S/C composite for enhanced lithium storage: mechanism and material properties. Chem Aust 1:733–740
Feng C, Huang L, Guo Z, Liu H (2007) Synthesis of tungsten disulfide (WS2) nanoflakes for lithium ion battery application. Electrochem Commun 9:119–122
Pham-Cong CJH, Yun J, Bandarenka AS, Kim J, Braun PV, Jeong SY, Cho CR (2016) Synergistically enhanced electrochemical performance of hierarchical MoS2/TiNb2O7 hetero-nanostructures as anode materials for li-ion batteries. ACS Nano 11:1026–1033
Tong X, Ashalley E, Lin F, Li H, Wang ZM (2015) Advances in MoS2-based field effect transistors (FETs). Nano-Micro Lett. 7:203–218
Perkgoz NK, Bay M (2016) Investigation of single-wall MoS2 monolayer flakes grown by chemical vapor deposition. Nano-Micro Lett 8:70–79
Hwang H, Kim H, Cho J (2011) MoS2 Nanoplates consisting of disordered graphene-like layers for high rate lithium battery anode materials. Nano Lett 11:4826
Jiang L, Lin B, Li X, Song X, Xia H, Li L, Zeng H (2016) Monolayer MoS2-graphene hybrid aerogels with controllable porosity for lithium-ion batteries with high reversible capacity. ACS Appl Mater Interfaces 8:2680–2687
Kong D, He H, Song Q, Wang B, Lv W, Yang Q, Zhi L (2014) Rational design of MoS2@graphene nanocables: towards high performance electrode materials for lithium ion batteries. Energy Environ Sci 7:3320–3325
Zhou J, Qin J, Zhang X, Shi C, Liu E, Zhao N, He C (2015) 2D space-confined synthesis of few-layer MoS2 anchored on carbon nanosheet for lithium-ion battery anode. ACS Nano 9:3837
Zhang S, Chowdari BV, Wen Z, Jin J, Yang J (2015) Constructing highly oriented configuration by few-layer MoS2: toward high-performance lithium-ion batteries and hydrogen evolution reactions. ACS Nano 9:12464–12472
Li J, Hou Y, Gao X, Guan D, Xie Y, Chen J, Yuan C (2015) A three-dimensionally interconnected carbon nanotube/layered MoS2 nanohybrid network for lithium ion battery anode with superior rate capacity and long-cycle-life. Nano Energy 16:10–18
Huang X, Zeng Z, Zhang H (2013) Metal dichalcogenide nanosheets: preparation, properties and applications. Chem Soc Rev 42:1934
Liu J, Fu A, Wang Y, Guo P, Feng H, Li H, Zhao XS (2017) Spraying coagulation-assisted hydrothermal synthesis of MoS2/carbon/graphene composite microspheres for lithium-ion battery applications. ChemElectroChem 4:2027-2036
Deng Z, Jiang H, Hu Y, Liu Y, Zhang L, Liu H, Li C (2017) 3D ordered macroporous MoS2@C nanostructure for flexible Li-ion batteries. Adv Mater 9:1603020
Zhao Z, Qin F, Kasiraju S, Xie L, Alam MK, Chen S, Wang D, Ren Z, Wang Z, Grabow LC (2017) Vertically aligned MoS2/Mo2C hybrid nanosheets grown on carbon paper for efficient electrocatalytic hydrogen evolution. ACS Catal 7:7312–7318
Chang K, Chen W (2011) L-cysteine-assisted synthesis of layered MoS2/graphene composites with excellent electrochemical performances for lithium ion batteries. ACS Nano 5:4720–4728
Shyyko LO, Kotsyubynsky VO, Budzulyak IM, Sagan P (2016) MoS2/C multilayer nanospheres as an electrode base for lithium power sources. Nanoscale Res Lett 11:243
Wang J-Z, Lu L, Lotya M, Coleman JN, Chou S-L, Liu H-K, Minett AI, Chen J (2013) Development of MoS2-CNT composite thin film from layered MoS2 for lithium batteries. Adv Energy Mater 3:798–805
Fu W, Du FH, Su J, Li XH, Wei X, Ye TN, Wang KX, Chen JS (2014) In situ catalytic growth of large-area multilayered graphene/MoS2 heterostructures. Sci Rep 4:4673
Zhang X, Zhao R, Wu Q, Li W, Shen C, Ni L, Yan H, Diao G, Chen M (2017) Petal-like MoS2 Nanosheets space-confined in hollow mesoporous carbon spheres for enhanced Lithium storage performance. ACS Nano 11:8429-8436
Beshkar F, Zinatloo-Ajabshir S, Salavati-Niasari M (2015) Simple morphology-controlled fabrication of nickel chromite nanostructures via a novel route. Chem Eng J 279:605–614
Vattikuti SVP, Chan B, Reddy CV, Shim J, Venkatesh B (2015) Co-precipitation synthesis and characterization of faceted MoS2 nanorods with controllable morphologies. Appl Phys A Mater Sci Process 119:813–823
Huang G, Liu Q, Kang W, Xing B, Chen L, Zhang C (2016) Potassium humate based reduced graphite oxide materials for supercapacitor applications. Electrochim Acta 196:450–456
Luo HM, Yang YF, Chen YZ, Zhang JQ, Zhao X (2015) Structure and electrochemical performance of highly porous carbons by single-step potassium humate carbonization for application in supercapacitors. J Appl Electrochem 46:1–9
Wang Z, Chen T, Chen W, Chang K, Ma L, Huang G, Chen D, Lee JY (2013) CTAB-assisted synthesis of single-layer MoS2-graphene composites as anode materials of li-ion batteries. J Mater Chem A 1:2202–2210
Choi M, Hwang J, Setiadi H, Chang W, Kim J (2017) One-pot synthesis of molybdenum disulfide-reduced graphene oxide (MoS2-RGO) composites and their high electrochemical performance as an anode in lithium ion batteries. J Supercrit Fluids 127:81–89
Yang W, He L, Tian X, Yan M, Yuan H, Liao X, Meng J, Hao Z, Mai L (2017) Carbon-MEMS-based alternating stacked MoS2@rGO-CNT micro-supercapacitor with high capacitance and energy density. Small 13:1700639
Liu Y, Ghosh R, Wu D, Ismach A, Ruoff R, Lai K (2014) Mesoscale imperfections in MoS2 atomic layers grown by a vapor transport technique. Nano Lett 14:4682
Zhao X, Hu C, Cao M (2013) Three-dimensional MoS2 hierarchical nanoarchitectures anchored into a carbon layer as graphene analogues with improved lithium ion storage performance. Chem Asian J 8:2701–2707
Jiang Y, Li X, Yu S, Jia L, Zhao X, Wang C (2015) Reduced graphene oxide-modified carbon nanotube/polyimide film supported MoS2 nanoparticles for electrocatalytic hydrogen evolution. Adv Funct Mater 25:2693–2700
Zhao S, Jin R, Song Y, Zhang H, House SD, Yang JC, Jin R (2017) Atomically precise gold nanoclusters accelerate hydrogen evolution over MoS2 nanosheets: the dual interfacial effect. Small 13:1701519
Wang J, Luo C, Gao T, Langrock A, Mignerey AC, Wang C (2015) An advanced MoS2/carbon anode for high-performance sodium-ion batteries. Small 11:473–481
Fang X, Yu X, Liao S, Shi Y, Hu YS, Wang Z, Stucky GD, Chen L (2012) Lithium storage performance in ordered mesoporous MoS2 electrode material. Microporous Mesoporous Mater 151:418–423
Chang K, Chen W (2011) Single-layer MoS2/graphene dispersed in amorphous carbon: towards high electrochemical performances in rechargeable lithium ion batteries. J Mater Chem 21:17175–17184
Du G, Guo Z, Wang S, Zeng R, Chen Z, Liu H (2010) Superior stability and high capacity of restacked molybdenum disulfide as anode material for lithium ion batteries. Chem Commun 46:1106–1108
The authors gratefully acknowledge the financial support given for this work by the National Natural Science Foundation of China, International Cooperation Project of Xinjiang Science and Technology Bureau, the Project of Xinjiang Education Office and National Program on Key Basic Research Project (973 Program).
This work was supported by the National Natural Science Foundation of China (U1503391, 51564045, 21566037, and 51272038), International Cooperation Project of Xinjiang Science and Technology Bureau (2017E0116 and 2017E01005), the Project of Xinjiang Education Office (XJEDU2017I004), and National Program on Key Basic Research Project (973 Program) 2013CB933301.
Availability of data and materials
The datasets supporting the conclusions of this article are included within the article and its additional files.
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Equations 1–5. The proposed reactions for the synthesis of MoS2. Table S1. The composition analysis of potassium humate. Figure S1. SEM images of (a) MoS2/C-600 and (b) MoS2/C-800 nanocomposite. Figure S2. High-resolution TEM image of MoS2/C-700 nanocomposite. Table S2. Comparison of electrochemical performance of MoS2-based electrodes. (DOC 2203 kb)
About this article
Cite this article
Geng, Q., Tong, X., Wenya, G.E. et al. Humate-assisted Synthesis of MoS2/C Nanocomposites via Co-Precipitation/Calcination Route for High Performance Lithium Ion Batteries. Nanoscale Res Lett 13, 129 (2018). https://doi.org/10.1186/s11671-018-2537-y
- MoS2/C nanocomposites
- Co-precipitation/calcination route
- Lithium-ion batteries